#------------------------------------------------------------------------------
#$Date: 2016-03-26 02:56:09 +0200 (Sat, 26 Mar 2016) $
#$Revision: 180161 $
#$URL: svn://www.crystallography.net/cod/cif/7/10/57/7105731.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7105731
loop_
_publ_author_name
'Andrea Alsobrook'
'Brad Hauser'
'Joseph Hupp'
'Evgeny V.Alekseev'
'Wulf Depmeier'
'Thomas Albrecht-Schmitt'
_publ_section_title
;
 Cubic and rhombohedral heterobimetallic networks constructed from
 uranium, transition metals, and phosphonoacetate: new methods for
 constructing porous materials
;
_journal_name_full               Chem.Commun.
_journal_page_first              9167
_journal_paper_doi               10.1039/c0cc03507f
_journal_volume                  46
_journal_year                    2010
_chemical_formula_moiety         Mn2[(UO2)6(PO3CH2CO2)3O3(OH)(H2O)2]*16H2O
_chemical_formula_sum            'C6 H42 Mn2 O49 P3 U6'
_chemical_formula_weight         2529.37
_chemical_name_systematic
;
?
;
_space_group_IT_number           204
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  '-I 2 2 3'
_symmetry_space_group_name_H-M   'I m -3'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            16
_cell_length_a                   26.4013(4)
_cell_length_b                   26.4013(4)
_cell_length_c                   26.4013(4)
_cell_measurement_reflns_used    3462
_cell_measurement_temperature    100(2)
_cell_measurement_theta_max      27.46
_cell_measurement_theta_min      2.18
_cell_volume                     18402.5(5)
_computing_cell_refinement       'SMART, SAINT'
_computing_data_collection       SMART
_computing_data_reduction        SAINT
_computing_molecular_graphics    'SHELXP-97 (Sheldrick, 1997)'
_computing_publication_material  'SHELXCIF-97 (Sheldrick, 2000)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      100(2)
_diffrn_detector_area_resol_mean 0
_diffrn_measured_fraction_theta_full 0.998
_diffrn_measured_fraction_theta_max 0.998
_diffrn_measurement_device_type  '0.3 /w exposure'
_diffrn_measurement_method       'BRUKER APEX'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0452
_diffrn_reflns_av_sigmaI/netI    0.0120
_diffrn_reflns_limit_h_max       34
_diffrn_reflns_limit_h_min       -34
_diffrn_reflns_limit_k_max       34
_diffrn_reflns_limit_k_min       -33
_diffrn_reflns_limit_l_max       34
_diffrn_reflns_limit_l_min       -33
_diffrn_reflns_number            110070
_diffrn_reflns_theta_full        27.46
_diffrn_reflns_theta_max         27.46
_diffrn_reflns_theta_min         2.18
_diffrn_standards_decay_%        0
_diffrn_standards_interval_count nm
_diffrn_standards_interval_time  nm
_diffrn_standards_number         nm
_exptl_absorpt_coefficient_mu    21.802
_exptl_absorpt_correction_T_max  0.309
_exptl_absorpt_correction_T_min  0.265
_exptl_absorpt_correction_type   numerical
_exptl_absorpt_process_details   SHELXPREP
_exptl_crystal_colour            orange
_exptl_crystal_density_diffrn    3.652
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             17872
_exptl_crystal_size_max          0.06280
_exptl_crystal_size_mid          0.05631
_exptl_crystal_size_min          0.05388
_refine_diff_density_max         1.607
_refine_diff_density_min         -1.205
_refine_diff_density_rms         0.150
_refine_ls_extinction_coef       0
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.090
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     237
_refine_ls_number_reflns         3759
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.090
_refine_ls_R_factor_all          0.0218
_refine_ls_R_factor_gt           0.0185
_refine_ls_shift/su_max          0.005
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0143P)²+263.6979P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0400
_refine_ls_wR_factor_ref         0.0411
_reflns_number_gt                3462
_reflns_number_total             3759
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            C0CC03507F.TXT
_cod_data_source_block           Mn2[(UO2)6(PO3CH2CO2)3O3(OH)(H2O)2]*16H2O
_cod_depositor_comments
;
The following automatic conversions were performed:

'_exptl_crystal_density_meas' value 'nm' was changed to '?' - the
value is perceived as not measured.

Automatic conversion script
Id: cif_fix_values 3008 2015-01-20 13:52:24Z robertas 
;
_cod_database_code               7105731
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, z'
'-x, y, -z'
'x, -y, -z'
'z, x, y'
'z, -x, -y'
'-z, -x, y'
'-z, x, -y'
'y, z, x'
'-y, z, -x'
'y, -z, -x'
'-y, -z, x'
'x+1/2, y+1/2, z+1/2'
'-x+1/2, -y+1/2, z+1/2'
'-x+1/2, y+1/2, -z+1/2'
'x+1/2, -y+1/2, -z+1/2'
'z+1/2, x+1/2, y+1/2'
'z+1/2, -x+1/2, -y+1/2'
'-z+1/2, -x+1/2, y+1/2'
'-z+1/2, x+1/2, -y+1/2'
'y+1/2, z+1/2, x+1/2'
'-y+1/2, z+1/2, -x+1/2'
'y+1/2, -z+1/2, -x+1/2'
'-y+1/2, -z+1/2, x+1/2'
'-x, -y, -z'
'x, y, -z'
'x, -y, z'
'-x, y, z'
'-z, -x, -y'
'-z, x, y'
'z, x, -y'
'z, -x, y'
'-y, -z, -x'
'y, -z, x'
'-y, z, x'
'y, z, -x'
'-x+1/2, -y+1/2, -z+1/2'
'x+1/2, y+1/2, -z+1/2'
'x+1/2, -y+1/2, z+1/2'
'-x+1/2, y+1/2, z+1/2'
'-z+1/2, -x+1/2, -y+1/2'
'-z+1/2, x+1/2, y+1/2'
'z+1/2, x+1/2, -y+1/2'
'z+1/2, -x+1/2, y+1/2'
'-y+1/2, -z+1/2, -x+1/2'
'y+1/2, -z+1/2, x+1/2'
'-y+1/2, z+1/2, x+1/2'
'y+1/2, z+1/2, -x+1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
U1 U 0.368223(8) 0.151088(8) 0.5000 0.00729(5) Uani 1 2 d S . .
U2 U 0.5000 0.136448(9) 0.569392(8) 0.01065(5) Uani 1 2 d S . .
U3 U 0.238374(6) 0.153871(6) 0.571742(6) 0.00892(4) Uani 1 1 d . . .
Mn1 Mn 0.31712(4) 0.31712(4) 0.68288(4) 0.0201(3) Uani 0.75 3 d SP . .
Mn2 Mn 0.2500 0.2500 0.7500 0.0207(4) Uani 1 6 d S . .
Mn3 Mn 0.35820(5) 0.0000 0.5000 0.0169(3) Uani 1 4 d S . .
P1 P 0.36764(4) 0.14336(4) 0.62424(4) 0.0097(2) Uani 1 1 d . . .
C1 C 0.38649(17) 0.19118(17) 0.66918(17) 0.0147(9) Uani 1 1 d . . .
H1AA H 0.4183 0.1815 0.6847 0.018 Uiso 1 1 calc R . .
H1BA H 0.3916 0.2231 0.6517 0.018 Uiso 1 1 calc R . .
C2 C 0.34654(16) 0.19805(17) 0.71009(16) 0.0127(8) Uani 1 1 d . . .
O1 O 0.23246(12) 0.22161(12) 0.56690(13) 0.0177(7) Uani 1 1 d . . .
O2 O 0.5000 0.1044(2) 0.65589(17) 0.0250(11) Uani 1 2 d S . .
O3 O 0.5000 0.20118(19) 0.58952(19) 0.0241(11) Uani 1 2 d S . .
O4 O 0.41169(11) 0.13346(13) 0.58788(12) 0.0182(7) Uani 1 1 d . . .
O5 O 0.24557(12) 0.08671(12) 0.57954(12) 0.0168(7) Uani 1 1 d . . .
O6 O 0.35073(12) 0.09778(12) 0.65347(11) 0.0158(6) Uani 1 1 d . . .
O7 O 0.33700(12) 0.16193(12) 0.73932(11) 0.0144(6) Uani 1 1 d . . .
O8 O 0.32636(11) 0.16519(12) 0.58933(11) 0.0139(6) Uani 1 1 d . . .
O9 O 0.18794(19) 0.1416(2) 0.5000 0.0301(13) Uani 1 2 d S . .
O10 O 0.5000 0.06982(18) 0.55659(17) 0.0180(10) Uani 1 2 d S . .
O11 O 0.37231(17) 0.21931(16) 0.5000 0.0151(9) Uani 1 2 d S . .
O12 O 0.45123(17) 0.15032(19) 0.5000 0.0174(10) Uani 1 2 d S . .
O13 O 0.36320(17) 0.08204(16) 0.5000 0.0142(9) Uani 1 2 d S . .
O14 O 0.28544(15) 0.15288(17) 0.5000 0.0124(9) Uani 1 2 d S . .
O15 O 0.32348(12) 0.23966(12) 0.71236(12) 0.0180(7) Uani 1 1 d . . .
OW1 O 0.2888(4) 0.0000 0.5398(4) 0.028(2) Uani 0.50 2 d SP . .
OW1A O 0.3120(4) 0.0000 0.5730(4) 0.023(2) Uani 0.50 2 d SP . .
OW2 O 0.3293(3) 0.2938(3) 0.6054(2) 0.103(3) Uani 1 1 d . . .
OW3 O 0.4158(4) 0.0000 0.5584(4) 0.096(4) Uani 1 2 d S . .
OW4 O 0.3658(7) 0.3658(7) 0.6342(7) 0.121(11) Uiso 0.50 3 d SP . .
OW5 O 0.5000 0.1546(3) 0.7412(2) 0.0451(17) Uani 1 2 d S . .
OW6 O 0.5255(5) 0.0000 0.6790(6) 0.068(4) Uani 0.60 2 d SP . .
OW7 O 0.2980(5) 0.2938(5) 0.5240(5) 0.091(4) Uiso 0.50 1 d P . .
OW8 O 0.4654(9) 0.2787(9) 0.5000 0.078(7) Uiso 0.40 2 d SP . .
OW9 O 0.4372(10) 0.2997(10) 0.4775(9) 0.054(6) Uiso 0.20 1 d P . .
OW10 O 0.4552(9) 0.3063(9) 0.6132(9) 0.062(6) Uiso 0.25 1 d P . .
OW11 O 0.5000 0.3001(15) 0.6156(15) 0.103(11) Uiso 0.30 2 d SP . .
OW12 O 0.4104(10) 0.3301(10) 0.4434(9) 0.091(7) Uiso 0.30 1 d P . .
OW13 O 0.3696(19) 0.3646(19) 0.4613(18) 0.132(17) Uiso 0.20 1 d P . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mn Mn 0.3368 0.7283 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
U U -9.6767 9.6646 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O11 U1 O13 179.3(2) . . ?
O11 U1 O14 92.19(18) . . ?
O13 U1 O14 87.08(18) . . ?
O11 U1 O12 87.10(19) . . ?
O13 U1 O12 93.63(19) . . ?
O14 U1 O12 179.29(18) . . ?
O11 U1 O4 98.66(10) . 26_556 ?
O13 U1 O4 81.67(10) . 26_556 ?
O14 U1 O4 116.11(7) . 26_556 ?
O12 U1 O4 64.03(7) . 26_556 ?
O11 U1 O4 98.66(10) . . ?
O13 U1 O4 81.67(10) . . ?
O14 U1 O4 116.11(7) . . ?
O12 U1 O4 64.03(7) . . ?
O4 U1 O4 123.82(13) 26_556 . ?
O11 U1 O8 83.33(9) . 26_556 ?
O13 U1 O8 96.36(9) . 26_556 ?
O14 U1 O8 64.98(7) . 26_556 ?
O12 U1 O8 114.92(7) . 26_556 ?
O4 U1 O8 54.37(9) 26_556 26_556 ?
O4 U1 O8 177.62(10) . 26_556 ?
O11 U1 O8 83.33(9) . . ?
O13 U1 O8 96.36(9) . . ?
O14 U1 O8 64.98(7) . . ?
O12 U1 O8 114.92(7) . . ?
O4 U1 O8 177.62(10) 26_556 . ?
O4 U1 O8 54.37(9) . . ?
O8 U1 O8 127.38(13) 26_556 . ?
O11 U1 P1 93.57(2) . 26_556 ?
O13 U1 P1 86.43(2) . 26_556 ?
O14 U1 P1 89.81(2) . 26_556 ?
O12 U1 P1 90.23(2) . 26_556 ?
O4 U1 P1 27.20(7) 26_556 26_556 ?
O4 U1 P1 150.64(7) . 26_556 ?
O8 U1 P1 27.40(7) 26_556 26_556 ?
O8 U1 P1 154.35(7) . 26_556 ?
O11 U1 P1 93.57(2) . . ?
O13 U1 P1 86.43(2) . . ?
O14 U1 P1 89.81(2) . . ?
O12 U1 P1 90.23(2) . . ?
O4 U1 P1 150.64(7) 26_556 . ?
O4 U1 P1 27.20(7) . . ?
O8 U1 P1 154.35(7) 26_556 . ?
O8 U1 P1 27.40(7) . . ?
P1 U1 P1 172.86(4) 26_556 . ?
O11 U1 U3 91.93(12) . 26_556 ?
O13 U1 U3 87.43(12) . 26_556 ?
O14 U1 U3 28.915(3) . 26_556 ?
O12 U1 U3 151.077(4) . 26_556 ?
O4 U1 U3 87.63(7) 26_556 26_556 ?
O4 U1 U3 144.27(7) . 26_556 ?
O8 U1 U3 36.52(6) 26_556 26_556 ?
O8 U1 U3 93.62(6) . 26_556 ?
P1 U1 U3 60.955(18) 26_556 26_556 ?
P1 U1 U3 118.663(19) . 26_556 ?
O11 U1 U3 91.93(12) . . ?
O13 U1 U3 87.43(12) . . ?
O14 U1 U3 28.915(3) . . ?
O12 U1 U3 151.077(4) . . ?
O4 U1 U3 144.27(7) 26_556 . ?
O4 U1 U3 87.63(7) . . ?
O8 U1 U3 93.62(6) 26_556 . ?
O8 U1 U3 36.52(6) . . ?
P1 U1 U3 118.663(19) 26_556 . ?
P1 U1 U3 60.955(18) . . ?
U3 U1 U3 57.830(5) 26_556 . ?
O3 U2 O10 173.6(2) . . ?
O3 U2 O12 94.91(19) . . ?
O10 U2 O12 90.35(17) . . ?
O3 U2 O12 94.91(19) . 3_656 ?
O10 U2 O12 90.35(17) . 3_656 ?
O12 U2 O12 69.15(18) . 3_656 ?
O3 U2 O4 88.32(9) . . ?
O10 U2 O4 90.35(9) . . ?
O12 U2 O4 67.39(12) . . ?
O12 U2 O4 136.54(12) 3_656 . ?
O3 U2 O4 88.32(9) . 28_655 ?
O10 U2 O4 90.35(9) . 28_655 ?
O12 U2 O4 136.54(12) . 28_655 ?
O12 U2 O4 67.39(12) 3_656 28_655 ?
O4 U2 O4 156.05(15) . 28_655 ?
O3 U2 O2 93.1(2) . . ?
O10 U2 O2 80.52(19) . . ?
O12 U2 O2 144.40(10) . . ?
O12 U2 O2 144.40(10) 3_656 . ?
O4 U2 O2 78.26(8) . . ?
O4 U2 O2 78.26(8) 28_655 . ?
O3 U2 U2 107.27(17) . 26_556 ?
O10 U2 U2 79.13(15) . 26_556 ?
O12 U2 U2 36.16(9) . 26_556 ?
O12 U2 U2 36.16(9) 3_656 26_556 ?
O4 U2 U2 101.82(7) . 26_556 ?
O4 U2 U2 101.82(7) 28_655 26_556 ?
O2 U2 U2 159.65(13) . 26_556 ?
O3 U2 U1 92.54(8) . . ?
O10 U2 U1 90.49(7) . . ?
O12 U2 U1 27.14(9) . . ?
O12 U2 U1 96.29(9) 3_656 . ?
O4 U2 U1 40.25(7) . . ?
O4 U2 U1 163.66(8) 28_655 . ?
O2 U2 U1 117.955(11) . . ?
U2 U2 U1 62.374(3) 26_556 . ?
O3 U2 U1 92.54(8) . 3_656 ?
O10 U2 U1 90.49(7) . 3_656 ?
O12 U2 U1 96.29(9) . 3_656 ?
O12 U2 U1 27.14(9) 3_656 3_656 ?
O4 U2 U1 163.66(8) . 3_656 ?
O4 U2 U1 40.25(7) 28_655 3_656 ?
O2 U2 U1 117.955(11) . 3_656 ?
U2 U2 U1 62.374(3) 26_556 3_656 ?
U1 U2 U1 123.424(6) . 3_656 ?
O5 U3 O1 177.25(16) . . ?
O5 U3 O14 91.51(15) . . ?
O1 U3 O14 89.98(15) . . ?
O5 U3 O9 90.90(19) . . ?
O1 U3 O9 91.79(19) . . ?
O14 U3 O9 68.50(13) . . ?
O5 U3 O6 90.93(13) . 44_455 ?
O1 U3 O6 89.39(13) . 44_455 ?
O14 U3 O6 140.17(12) . 44_455 ?
O9 U3 O6 71.71(12) . 44_455 ?
O5 U3 O8 89.91(13) . . ?
O1 U3 O8 88.50(13) . . ?
O14 U3 O8 68.31(11) . . ?
O9 U3 O8 136.81(12) . . ?
O6 U3 O8 151.45(10) 44_455 . ?
O5 U3 O7 89.10(13) . 44_455 ?
O1 U3 O7 88.37(13) . 44_455 ?
O14 U3 O7 145.81(11) . 44_455 ?
O9 U3 O7 145.68(12) . 44_455 ?
O6 U3 O7 73.97(11) 44_455 44_455 ?
O8 U3 O7 77.51(10) . 44_455 ?
O5 U3 U3 96.59(10) . 26_556 ?
O1 U3 U3 85.92(11) . 26_556 ?
O14 U3 U3 33.27(9) . 26_556 ?
O9 U3 U3 35.89(10) . 26_556 ?
O6 U3 U3 107.03(8) 44_455 26_556 ?
O8 U3 U3 101.22(7) . 26_556 ?
O7 U3 U3 174.19(8) 44_455 26_556 ?
O5 U3 U1 86.81(10) . . ?
O1 U3 U1 93.45(10) . . ?
O14 U3 U1 27.81(9) . . ?
O9 U3 U1 95.98(10) . . ?
O6 U3 U1 167.46(8) 44_455 . ?
O8 U3 U1 40.98(7) . . ?
O7 U3 U1 118.28(7) 44_455 . ?
U3 U3 U1 61.085(3) 26_556 . ?
OW2 Mn1 OW2 99.9(3) . 8_656 ?
OW2 Mn1 OW2 99.9(3) . 11_566 ?
OW2 Mn1 OW2 99.9(3) 8_656 11_566 ?
OW2 Mn1 O15 88.0(2) . 11_566 ?
OW2 Mn1 O15 163.1(3) 8_656 11_566 ?
OW2 Mn1 O15 93.3(2) 11_566 11_566 ?
OW2 Mn1 O15 93.3(2) . . ?
OW2 Mn1 O15 88.0(2) 8_656 . ?
OW2 Mn1 O15 163.1(3) 11_566 . ?
O15 Mn1 O15 76.59(14) 11_566 . ?
OW2 Mn1 O15 163.1(3) . 8_656 ?
OW2 Mn1 O15 93.3(2) 8_656 8_656 ?
OW2 Mn1 O15 88.0(2) 11_566 8_656 ?
O15 Mn1 O15 76.59(14) 11_566 8_656 ?
O15 Mn1 O15 76.59(14) . 8_656 ?
OW2 Mn1 OW4 62.1(2) . . ?
OW2 Mn1 OW4 62.1(2) 8_656 . ?
OW2 Mn1 OW4 62.1(2) 11_566 . ?
O15 Mn1 OW4 134.31(9) 11_566 . ?
O15 Mn1 OW4 134.31(9) . . ?
O15 Mn1 OW4 134.31(9) 8_656 . ?
OW2 Mn1 Mn2 117.9(2) . . ?
OW2 Mn1 Mn2 117.9(2) 8_656 . ?
OW2 Mn1 Mn2 117.9(2) 11_566 . ?
O15 Mn1 Mn2 45.69(9) 11_566 . ?
O15 Mn1 Mn2 45.69(9) . . ?
O15 Mn1 Mn2 45.69(9) 8_656 . ?
OW4 Mn1 Mn2 180.0(4) . . ?
O15 Mn2 O15 180.00(17) 44_455 8_656 ?
O15 Mn2 O15 103.51(13) 44_455 11_566 ?
O15 Mn2 O15 76.49(13) 8_656 11_566 ?
O15 Mn2 O15 103.51(13) 44_455 . ?
O15 Mn2 O15 76.49(13) 8_656 . ?
O15 Mn2 O15 76.49(13) 11_566 . ?
O15 Mn2 O15 76.49(13) 44_455 37_556 ?
O15 Mn2 O15 103.51(13) 8_656 37_556 ?
O15 Mn2 O15 103.51(13) 11_566 37_556 ?
O15 Mn2 O15 180.000(1) . 37_556 ?
O15 Mn2 O15 76.49(13) 44_455 47_545 ?
O15 Mn2 O15 103.51(13) 8_656 47_545 ?
O15 Mn2 O15 180.000(1) 11_566 47_545 ?
O15 Mn2 O15 103.51(13) . 47_545 ?
O15 Mn2 O15 76.49(13) 37_556 47_545 ?
O15 Mn2 Mn1 134.37(8) 44_455 . ?
O15 Mn2 Mn1 45.63(8) 8_656 . ?
O15 Mn2 Mn1 45.63(8) 11_566 . ?
O15 Mn2 Mn1 45.63(8) . . ?
O15 Mn2 Mn1 134.37(8) 37_556 . ?
O15 Mn2 Mn1 134.37(8) 47_545 . ?
O15 Mn2 Mn1 45.63(8) 44_455 37_556 ?
O15 Mn2 Mn1 134.37(8) 8_656 37_556 ?
O15 Mn2 Mn1 134.37(8) 11_566 37_556 ?
O15 Mn2 Mn1 134.37(8) . 37_556 ?
O15 Mn2 Mn1 45.63(8) 37_556 37_556 ?
O15 Mn2 Mn1 45.63(8) 47_545 37_556 ?
Mn1 Mn2 Mn1 180.00(3) . 37_556 ?
OW1 Mn3 OW1 59.7(7) 26_556 . ?
OW1 Mn3 OW3 104.8(5) 26_556 26_556 ?
OW1 Mn3 OW3 164.4(5) . 26_556 ?
OW1 Mn3 OW3 164.4(5) 26_556 . ?
OW1 Mn3 OW3 104.8(5) . . ?
OW3 Mn3 OW3 90.8(7) 26_556 . ?
OW1 Mn3 O13 93.03(11) 26_556 . ?
OW1 Mn3 O13 93.03(11) . . ?
OW3 Mn3 O13 87.55(9) 26_556 . ?
OW3 Mn3 O13 87.55(9) . . ?
OW1 Mn3 O13 93.03(11) 26_556 27 ?
OW1 Mn3 O13 93.03(11) . 27 ?
OW3 Mn3 O13 87.55(9) 26_556 27 ?
OW3 Mn3 O13 87.55(9) . 27 ?
O13 Mn3 O13 173.0(2) . 27 ?
OW1 Mn3 OW1A 27.8(4) 26_556 26_556 ?
OW1 Mn3 OW1A 87.5(5) . 26_556 ?
OW3 Mn3 OW1A 76.9(4) 26_556 26_556 ?
OW3 Mn3 OW1A 167.7(4) . 26_556 ?
O13 Mn3 OW1A 91.86(7) . 26_556 ?
O13 Mn3 OW1A 91.86(7) 27 26_556 ?
OW1 Mn3 OW1A 87.5(5) 26_556 . ?
OW1 Mn3 OW1A 27.8(4) . . ?
OW3 Mn3 OW1A 167.7(4) 26_556 . ?
OW3 Mn3 OW1A 76.9(4) . . ?
O13 Mn3 OW1A 91.86(7) . . ?
O13 Mn3 OW1A 91.86(7) 27 . ?
OW1A Mn3 OW1A 115.4(6) 26_556 . ?
O6 P1 O4 114.36(19) . . ?
O6 P1 O8 113.47(18) . . ?
O4 P1 O8 103.08(17) . . ?
O6 P1 C1 107.82(19) . . ?
O4 P1 C1 108.83(19) . . ?
O8 P1 C1 109.1(2) . . ?
O6 P1 U1 124.44(13) . . ?
O4 P1 U1 51.76(12) . . ?
O8 P1 U1 51.87(12) . . ?
C1 P1 U1 127.74(15) . . ?
C2 C1 P1 111.1(3) . . ?
C2 C1 H1AA 109.4 . . ?
P1 C1 H1AA 109.4 . . ?
C2 C1 H1BA 109.4 . . ?
P1 C1 H1BA 109.4 . . ?
H1AA C1 H1BA 108.0 . . ?
O7 C2 O15 122.6(4) . . ?
O7 C2 C1 119.1(4) . . ?
O15 C2 C1 118.3(4) . . ?
P1 O4 U2 150.01(19) . . ?
P1 O4 U1 101.05(15) . . ?
U2 O4 U1 103.91(11) . . ?
P1 O6 U3 137.96(19) . 47_545 ?
C2 O7 U3 137.0(3) . 47_545 ?
P1 O8 U3 139.32(18) . . ?
P1 O8 U1 100.74(15) . . ?
U3 O8 U1 102.51(11) . . ?
U3 O9 U3 108.2(2) . 26_556 ?
U1 O12 U2 124.68(10) . . ?
U1 O12 U2 124.68(10) . 26_556 ?
U2 O12 U2 107.69(18) . 26_556 ?
U1 O13 Mn3 179.3(3) . . ?
U1 O14 U3 123.27(9) . 26_556 ?
U1 O14 U3 123.27(9) . . ?
U3 O14 U3 113.46(17) 26_556 . ?
C2 O15 Mn1 146.5(3) . . ?
C2 O15 Mn2 123.9(3) . . ?
Mn1 O15 Mn2 88.69(12) . . ?
OW1A OW1 Mn3 84.9(8) . . ?
OW1 OW1A Mn3 67.2(7) . . ?
OW9 OW8 OW9 65(3) . 26_556 ?
OW8 OW9 OW9 57.3(15) . 26_556 ?
OW8 OW9 OW12 168(3) . . ?
OW9 OW9 OW12 130.1(15) 26_556 . ?
OW11 OW10 OW13 91(3) . 31_556 ?
OW10 OW11 OW10 163(5) . 28_655 ?
OW9 OW12 OW13 121(3) . . ?
OW12 OW13 OW10 149(4) . 34_565 ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
U1 O11 1.804(4) . ?
U1 O13 1.828(4) . ?
U1 O14 2.186(4) . ?
U1 O12 2.192(4) . ?
U1 O4 2.630(3) 26_556 ?
U1 O4 2.630(3) . ?
U1 O8 2.631(3) 26_556 ?
U1 O8 2.631(3) . ?
U1 P1 3.2865(10) 26_556 ?
U1 P1 3.2865(10) . ?
U1 U3 3.9173(2) 26_556 ?
U1 U3 3.9173(2) . ?
U2 O3 1.790(5) . ?
U2 O10 1.791(5) . ?
U2 O12 2.269(3) . ?
U2 O12 2.269(3) 3_656 ?
U2 O4 2.383(3) . ?
U2 O4 2.383(3) 28_655 ?
U2 O2 2.436(5) . ?
U2 U2 3.6641(4) 26_556 ?
U2 U1 3.9509(2) 3_656 ?
U3 O5 1.795(3) . ?
U3 O1 1.800(3) . ?
U3 O14 2.265(2) . ?
U3 O9 2.338(3) . ?
U3 O6 2.348(3) 44_455 ?
U3 O8 2.388(3) . ?
U3 O7 2.393(3) 44_455 ?
U3 U3 3.7882(3) 26_556 ?
Mn1 OW2 2.160(6) . ?
Mn1 OW2 2.160(6) 8_656 ?
Mn1 OW2 2.160(6) 11_566 ?
Mn1 O15 2.194(3) 11_566 ?
Mn1 O15 2.194(3) . ?
Mn1 O15 2.194(3) 8_656 ?
Mn1 OW4 2.23(3) . ?
Mn1 Mn2 3.0692(17) . ?
Mn2 O15 2.197(3) 44_455 ?
Mn2 O15 2.197(3) 8_656 ?
Mn2 O15 2.197(3) 11_566 ?
Mn2 O15 2.197(3) . ?
Mn2 O15 2.197(3) 37_556 ?
Mn2 O15 2.197(3) 47_545 ?
Mn2 Mn1 3.0692(17) 37_556 ?
Mn3 OW1 2.112(10) 26_556 ?
Mn3 OW1 2.112(10) . ?
Mn3 OW3 2.167(7) 26_556 ?
Mn3 OW3 2.167(7) . ?
Mn3 O13 2.170(4) . ?
Mn3 O13 2.170(4) 27 ?
Mn3 OW1A 2.282(10) 26_556 ?
Mn3 OW1A 2.282(10) . ?
P1 O6 1.498(3) . ?
P1 O4 1.530(3) . ?
P1 O8 1.539(3) . ?
P1 C1 1.803(5) . ?
C1 C2 1.520(6) . ?
C1 H1AA 0.9700 . ?
C1 H1BA 0.9700 . ?
C2 O7 1.252(5) . ?
C2 O15 1.257(5) . ?
O6 U3 2.348(3) 47_545 ?
O7 U3 2.393(3) 47_545 ?
O9 U3 2.338(3) 26_556 ?
O12 U2 2.269(3) 26_556 ?
O14 U3 2.265(2) 26_556 ?
OW1 OW1A 1.070(15) . ?
OW6 OW6 1.34(3) 2_655 ?
OW7 OW7 1.27(3) 26_556 ?
OW8 OW9 1.10(3) . ?
OW8 OW9 1.10(3) 26_556 ?
OW9 OW9 1.19(5) 26_556 ?
OW9 OW12 1.40(3) . ?
OW10 OW11 1.20(2) . ?
OW10 OW13 1.78(5) 31_556 ?
OW11 OW10 1.20(2) 28_655 ?
OW12 OW13 1.49(5) . ?
OW13 OW10 1.78(5) 34_565 ?
